HAL Id: hal-01401907
Submitted on 24 Nov 2016
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Distributed under a Creative Commons Attribution| 4.0 International License
Analytical modeling of synthetic fiber ropes subjected to
axial loads. Part I: A new continuum model for
multilayered fibrous structures
Seyed Reza Ghoreishi, Patrice Cartraud, Peter Davies, Tanguy Messager
To cite this version:
Seyed Reza Ghoreishi, Patrice Cartraud, Peter Davies, Tanguy Messager. Analytical modeling of
synthetic fiber ropes subjected to axial loads. Part I: A new continuum model for multilayered
fi-brous structures. International Journal of Solids and Structures, Elsevier, 2007, 44 (9), pp.2924-2942.
Analytical modeling of synthetic ﬁber ropes subjected
to axial loads. Part I: A new continuum model
for multilayered ﬁbrous structures
Institut de recherche en Ge´nie civil et Me´canique (Ge´M), Ecole Centrale de Nantes, 1, Rue de la Noe, BP92101, 44321 Nantes Cedes 03, France
IFREMER, Materials and Structures group BP70, 29280 Plouzane´, France c
Universite´ de Nantes, Nantes Atlantique Universite´s, Institut de recherche en Ge´nie civil et Me´canique (Ge´M), Ecole Centrale de Nantes, BP92101, 44321 Nantes, France
Synthetic ﬁber ropes are characterized by a very complex architecture and a hierarchical structure. Considering the ﬁber rope architecture, to pass from ﬁber to rope structure behavior, two scale transition models are necessary, used in sequence: one is devoted to an assembly of a large number of twisted components (multilayered), whereas the second is suitable for a structure with a central straight core and six helical wires (1 + 6). The part I of this paper ﬁrst describes the development of a model for the static behavior of a ﬁbrous structure with a large number of twisted components. Tests were then performed on two diﬀerent structures subjected to axial loads. Using the model presented here the axial stiﬀness of the structures has been predicted and good agreement with measured values is obtained. A companion paper presents the second model to predict the mechanical behavior of a 1 + 6 ﬁbrous structure.
Keywords: Fiber rope; Yarn; Aramid; Multilayered structures; Analytical model; Testing
Synthetic ﬁber rope mooring systems, which are often composed of steel chain at the ends and a central synthetic ﬁber rope, are increasingly ﬁnding applications as oﬀshore oil exploration goes to deeper sites. Pre-vious researchers have shown that such mooring lines provide numerous advantages over steel mooring lines
(steel wire ropes and chains), particularly in deep water applications for which the large self-weight of steel lines is prohibitive (Beltran and Williamson, 2004; Foster, 2002). It is therefore essential to be able to model the mechanical behavior of very long synthetic mooring lines in order to reduce the need for expensive tests under varying parameters and operating conditions.
Large synthetic ﬁber ropes are assemblies of millions of ﬁbers and characterized by a very complex archi-tecture and a hierarchical structure in which the base components (ﬁber or yarn) are modiﬁed by twisting operations. This structure is then a base component for the next higher structure. Its hierarchical structure leads to the hierarchical approach where the top is the ﬁber rope and the bottom is the base components, with several diﬀerent types of elements between the base component and the ﬁber rope, i.e. yarn, assembled yarn and strand. Fig. 1 illustrates this hierarchical structure.
Considering the ﬁber rope architecture, it consists of two diﬀerent types of structure: one is a structure with a central straight core and six helical components (1 + 6), whereas the second is an assembly of a large number of twisted components (multilayered), see Fig. 2. So to pass from ﬁber to rope structure, two scale transition models are necessary, used in sequence. The results of the model at each level can be used as input data for the model at the next higher level. Use of this approach from the lowest level, at which mechanical properties are given as input, to the highest level of the rope determines the rope properties. Based on this strategy, the tran-sition models can be used to analyze synthetic ﬁber ropes of complex cross-section. Fig. 3 shows the typical hierarchy ranking from the smallest level to the highest level for a 205 ton break load ﬁber rope.
The focus of this paper is the modeling of the static behavior of a ﬁbrous structure with a large number of twisted components subjected to axial loads, starting from the mechanical behavior of the base component, and the geometric description of the rope structure.
Cross section A-A
Strand Assembled yarn
Fig. 1. Synthetic ﬁber rope structure. (a) Fiber robe with 1 + 6 strands and (b) construction of a strand.
Fig. 2. Cross-section of a synthetic ﬁber rope (205 ton break load); the rope represents a 1 + 6 structure, core and strands are assemblies of a large number of twisted components.
In Section 2, a description of the structure (geometry and behavior) is given, then, in Section 3, we present an overview of the existing mechanical models of such structures. In Section 4, a new continuum model is developed. The analytical models are compared in Section 5. Tensile tests have been performed, to provide the experimental data that are described in Section 6. In Section 7, we demonstrate the accuracy of the models by comparing their predictions to experimental results.
2. Structure description
Let us consider a multilayered structure in which each component follows a regular helical path round a central axis of the structure. The geometry of each component is characterized by the pitch length, P (length of one turn of the twist, or reciprocal of twists per unit length) and the lay angle, a, measured with respect to the structure Z axis. The component’s centerline is then an helical curve of radius r.
The pitch length P, is the same at all radial positions, but the lay angle will increase from zero at the center
to a maximum at the external surface of the structure, ae, as shown in Fig. 4.
It may be noted that the component cross-sections are elliptical in the plane perpendicular to the Z axis.
Therefore, the lay angle of a component at a radial position ri, denoted by aican be calculated using the
fol-lowing expression: Yar n stiffness Model 1 Assembled yarns geometry Model 1 Strands geometry Rope geometry
Assembled Yarn stiffness
Rope stiffness matrix
Rope Model 2
Model 1: for a structure with a large number of components. Model 2: for a 1+6 structure.
For marine applications, the ﬁber ropes are subjected to axial loads, and the axial behavior of such structures exhibits coupling between tension and torsion due to the helical design of the components. Thus, the overall behavior can be expressed in the form:
Fz Mz ¼ kee keh khe khh u z;z hz;z ð2Þ
where uz,zdenotes the overall axial strain, hz,zthe twist angle per unit length, Fzthe axial force and Mzthe
torque. The four stiﬀness matrix components kee, khh, kheand kehare pure tensile, pure torsion and coupling
terms respectively. Moreover, the stiﬀness matrix should be symmetric, as can be shown from Betti’s reciprocal theorem.
3. Earlier models
This work is concentrated on structures with a large number of components (constitutive elements). As noted by Raoof and Hobbs (1988), since the structure consists of a large number of components, the bending moments and torque in individual components can be neglected. Several authors have developed analytical models to predict the global elastic constants providing the relationship between loads and strains for such multilayered structures, based on a knowledge of the component material and geometry of the structure.
Two categories of these models are presented: semi-continuous models developed for metallic cables and models speciﬁcally presented for synthetic cables.
3.1. Semi-continuous models
Homogenization is a well known method in solid mechanics, and can be used for the continuum mod-eling of a discrete system composed of a large number of identical repetitive elements. With an appropriate
choice of the material parameters, one can accurately represent the global behavior of the real system. This method was ﬁrst applied to cable modeling by Hobbs and Raoof (1982). It is the orthotropic sheet model that has been described in detail by Raoof (1983) and then extended by Raoof and his associates over two decades.
In this model the classical twisted rod theories for the behavior of helical laid wires has been extended to include a set of kinematic compatibility conditions. The individual layer of wires is replaced by an equivalent cylindrical orthotropic sheet, which is assumed to be thin and to be in a plane stress state.
As in the case of composite laminates, four elastic constants are necessary. Two of them are obtained directly from the mechanical properties of the wires. The other two are related to the contact stiﬀness between adjacent wires in the layer. The complete structure is then treated as a discrete set of concentric orthotropic cylinders. The orthotropy axes correspond to those of a ﬁber composite material in which the ﬁbers have the same lay angle as the wires in the corresponding layer.
Another semi-continuous model was developed by Blouin and Cardou (1989), and later extended by Jolic-oeur and Cardou (1994, 1996). This also consists of replacing each layer with a cylinder of orthotropic, trans-versely isotropic material. In this model the elastic constants can be used as free, adjustable, parameters, or else estimated rationally from contact mechanics equations as in the case of the orthotropic sheet model.
Once the cable is modeled using such continuum approach, analytical solutions for elementary loadings can be derived (Crossley et al., 2003a,b).
These semi-continuous models take into account friction between constituents. However, some elastic con-stants are obtained from contact mechanics, considering layer components have circular cross-section. It can be seen from Fig. 2 that this is not the case for ﬁber ropes. Moreover, due to the homogenization process, the accuracy of this model increases when the number of wires in a given layer increases. Lastly, these models are tedious to use, and since they are non-linear, they require numerical solving.
Despite these limitations, the model of Raoof and Hobbs (1988), brieﬂy presented in Section 3.3, will be applied here in section 5.
3.2. Synthetic ﬁber ropes models
In this category the simplest model is that of Hoppe (1991) in which the structure and the components are assumed to be subjected to pure tensile forces, the bending and torsional stiﬀness for both of them being neglected. Contact and friction between the components are also neglected, but such an approximation is jus-tiﬁed for monotonic axial loading. It should be noted that this analytical model provides only the overall ten-sile behavior.
Leech et al. (1993), presented a more complex quasi-static analysis of ﬁber ropes and included it in a com-mercial software: ﬁber rope modeller or FRM (2003). Their analysis is based on the principle of virtual work and can take frictional eﬀects into account. The program computes tension and torque from their dependence on elongation and twist.
Another model was developed by Rungamornrat et al. (2002), and later extended by Beltran et al. (2003) and Beltran and Williamson (2004). These models are very similar with that of Leech but they have concen-trated on a damage model to take into account the degradation of rope properties as a function of loading history.
Leech’s model appears to be very sophisticated, with an accurate mechanical modeling of the components of the ﬁber ropes behavior and their interactions. Moreover, the cross-section geometry can be described using diﬀerent forms of arrangement of components (see Section 3.5). Therefore, Leech’s model can be considered as a reference model, but it requires resolution.
Hereafter, the synthetic ﬁber ropes models of Hoppe (1991) and Leech et al. (1993) are brieﬂy presented and then a new continuum model will be developed from the Hoppe’s one to analysis the structure with a large number of twisted components.
3.3. Raoof’s model
Raoof and his associates have worked extensively on the behavior of metallic structures with a large num-ber of wires so that the bending moments and torque in individual wires become much less signiﬁcant than
they are in six and seven wire cables (Hobbs and Raoof, 1982; Raoof, 1983; Raoof and Hobbs, 1988; Raoof, 1991; Raoof and Kraincanic, 1995a; Raoof and Kraincanic, 1995b). In these studies a great deal of attention has been paid to the inter-wire contact phenomena and friction has been taken fully into account. By treating each layer of wires as an orthotropic sheet with non-linear properties determined using the mechanical contact theories and assuming Coulomb friction, it has been possible to establish the stiﬀness matrix in the presence of an axial load.
The main features of this model are presented hereafter, in the case of metallic multilayered structure with an isotropic material.
These authors have established a set of non-linear simultaneous equations to analyse the kinematics of each layer of wires, providing a set of compatible strains in the anisotropic cylinder with a core (for more details see Raoof and Hobbs (1988)). The elastic behavior of each orthotropic sheet in the local coordinate system (t, b, n), see Fig. 5, can be expressed in the following matrix form:
ett ebb etb 8 > < > : 9 > = > ;¼ S11 S12 0 S12 S22 0 0 0 S66 8 > < > : 9 > = > ; rtt rbb rtb 8 > < > : 9 > = > ; ð3Þ
where Sij, e and r are the compliance, the strains and stresses referred to the axes of orthotropy parallel and
normal to the wire axes, respectively.
The compliance parallel to the wire axis S11is straightforward, reﬂecting the ratio between the sheet area
and the wire area (4/p): S11¼
where E is the Young’s modulus for the wire material, and the coupling term S12is given by
S12¼ mS11 ð5Þ
where m is Poisson’s ratio.
The compression compliance, S22, has been expressed as S22¼ 1 pE 4ð1 m 2Þ 1 3þ ln 1:25D PcDð1m2Þ E 1=2 2 6 4 3 7 5 2ð1 m2Þ 0 B @ 1 C A ð6Þ
where D is the wire diameter and, Pcis the contact load per unit length on the contact area which is obtained
from Hertzian contact theory for the contact of two parallel cylinders. The contact load, Pc, is determined
numerically by using an iterative method.
The shear compliance, S66, is determined from other results of the contact theory (Mindlin, 1949):
S66¼ S22 1 m 1 dl dlmax 1=2 ð7Þ where dlis the line contact displacement for a given total perturbation in structure axial strain, and dl maxis the
corresponding displacement at the onset of full-sliding condition.
The stiﬀness (or compliance) has been shown to be a function of the amplitude of the load variation about the mean. For small changes of axial force the stiﬀness is larger than it is for bigger variations. Small changes do not overcome the inter-wire friction, while larger changes do, causing sliding and a lower eﬀective modulus. In this study, the stiﬀness matrix results of this model for two extreme cases are presented: the lower bound
or full-slip, correspond to dl= dl max and the upper bound or no-slip for dl= 0.
Once the stiﬀness matrix of all the layers (for a given axial preload) has been found, in order to obtain the behavior of the structure, the stiﬀness matrix of each layer is transformed into the global coordinate system of the structure (t0, b0, n0), see Fig. 5, and the summation of the stiﬀness of all the layers enables the global
behav-ior of the structure to be established.
It should be noted that to apply this model to a multilayered ﬁbrous structure, Young’s modulus of the component material is obtained from axial stiﬀness of components in the direction of their axis, see section 4. In addition, Poisson’s ratio, m, according to the volume constant deformation assumption, has been set to 0.5.
3.4. Hoppe’s model
The work of Hoppe (1991) based on purely geometrical considerations, allows a model of behavior of this type of structure under a simple tensile force to be determined. This model requires the knowledge of the ten-sile properties of the components and the construction parameters of the structure, i.e. the number of layers, the number of components in each layer and the lay angle of each layer. This model is based on the following hypotheses: the geometry of the structure is multilayered with the helical component having circular section; at the local and global levels, the base components and the structure work only in traction in the direction of their axis (bending and torsion are neglected); the section of the structure remains plane, and perpendicular to its axis after deformation; deformation of the structure is at constant volume; strains and friction eﬀects due to contact between components are neglected.
Using these hypotheses, the elongation of each component is determined as a function of those of the struc-ture, and then the axial force in each component is determined. The projection of the force on the structure axis and summing for all the components enables a closed-form expression for the global behavior (only axial stiﬀness) of the structure to be established. In section 4, a closed-form analytical solution, for stiﬀness matrix components, will be developed which is based on Hoppe’s model.
3.5. Leech’s model
Leech et al. (1993) presented a model whose formulation is based on the principle of virtual work to ana-lyze ﬁber ropes. This model is integrated in a commercial software (FRM, 2003) to predict the behavior of the synthetic cables subjected to an axial load. This model diﬀers from Hoppe’s model by the following aspects: at the global level, the behavior of the structure is characterized by coupling between tension and
between components are considered; the geometry of the structure is multilayered, and two extreme rope geometry descriptions in transverse deformation have been considered: Layered packing geometry and Wedge geometry, see Fig. 6.
For layered packing geometry, it is assumed that a bundle of parallel identical components with circular cross-section is twisted in the assembly to form a structure with a core, surrounded by a layer of equally wound components, this layer enclosed by another layer and so on until all the components are used. Each layer is a helical structure of many components and each helix has the same pitch length but a diﬀerent lay angle.
For wedge geometry, the components in the same level are allowed to deform transversely and change their shape to a wedge or truncated wedge. The equivalent helix radius is the radius of the center of area of the wedge. Within each layer the packing factor (PF) is introduced to take into account the presence of the voids in the layer that can be deﬁned by the ratio of the area of material to the layer cross-sectional area. It can be expressed by
where ni, Acand Wiare the number of components in layer i, component cross-section area and the width of
the layer i respectively. It should be noted that for a given PF, the width of the layer will be deﬁned and vice versa.
The estimation of the frictional forces that develop between the components in a structure is based on the classical slip-stick model where the friction force is assumed to develop between two contact surfaces in the direction opposite to the relative slip of these two surfaces. Six sliding modes have been presented and it was noted that, for the twisted structure under axial loading, the only signiﬁcant frictional contribution (and even that is small) comes from the axial sliding mode (Leech et al., 1993; Leech, 2002).
In the present study, FRM software was used to obtain the results for Leech’s model, with the wedge geom-etry option. First, the structure is deﬁned. Essentially, this consists of specifying the number of components in each layer with the appropriate twist and the nature of the packing at that layer. Second, the dimensional and tensile properties of the components must be provided. Most are single parameters, but the non-linear force– strain relations can be deﬁned in the software by the coeﬃcients of fourth order polynomials. In this study the force–strain relations were considered linear and derived from test data.
The stiﬀness matrix is obtained in two steps. First, we let hz,z= 0 and vary the axial strain, uz,z, about a
given value (0.01), to calculate Fzand Mz through the FRM software, which leads to keeand khe from Eq.
(1). In the same way, kehand khhwill be obtained by setting to 0 the axial strain, uz,z, and varying hz,z.
Fig. 6. Multilayered geometry of structure for various models: (a) Raoof, Hoppe and Leech (layered packing geometry) and (b) Leech (wedge geometry).
4. Continuum model
All the models presented above require the construction parameters of the structure such as number of lay-ers, number of components in each layer (see Fig. 6) and lay angle of each layer (see Fig. 5). These are not always easy to deﬁne precisely for ﬁber rope structures, see Fig. 2, where it appears diﬃcult to model the strand cross-section as a multilayered structure. In addition, these models are integrated in programs and numerical analysis is necessary (except for the Hoppe model which presented a closed-form expression but only for the pure tensile behavior of the structure with no torsion and coupling terms).
Here, an analytical model with a closed-form expression and model geometry more in agreement with the real geometry of the structure will be established. This involves an extension of Hoppe’s model (Hoppe, 1991) which is based on the same hypotheses, as in the initial model, with an exception which is detailed in the next paragraph.
In the literature, the structures are described using a multilayered geometry, but in the present model we do not consider them like an assembly of layers, but rather as a continuum formed by a set of coaxial helixes. These helixes have the same number of turns per unit length, and their section amounts to a material point, and that describe the geometry of a constituent element. It is in this sense that this model is termed a contin-uum model. Moreover, within the structure the packing is assumed to be uniform. Therefore, the geometric input data for this model are restricted to the external structure radius, the pitch length and a packing factor value. In addition, the present model can describe coupling behavior between traction and torsion.
The stress–strain (force–strain) properties of the material which are introduced into the model are, in general, taken to correspond to the actual force–strain properties of the component as obtained from experiments. The relation between force–strain is assumed linear and Young’s modulus of the component material is given by
Ec¼ kc=Ac ð9Þ
where kcis the component axial stiﬀness (slope of the force–strain curve) and Acis the cross-section area of the
4.1. Axial strain of components
In the present model, the components are assumed to be subjected to pure tensile forces, the bending and torsion stiﬀness are neglected. In axial loading, with traction and torsion, the axial strain of each component is composed of two diﬀerent parts: the ﬁrst results from the elongation of the structure, whereas the second is due to its rotation. For small strains, it is possible to separate these phenomena, the axial deformation of the component is expressed therefore by
ett ¼ eAtt þ e R
where t is the tangent to the component center line, eA
ttand e R
tt are the axial strains of the component due to the
elongation and to the rotation of the structure respectively. 4.1.1. Elongation
Let kzbe the extension ratio (ratio of deformed length to initial length of the structure) measured along the
structure axis, and krthe corresponding extension ratio for a component whose initial and ﬁnal radial
posi-tions are r0and r, respectively, see Fig. 7(a). The extension ratios, kzand kr, are deﬁned as follows:
kz¼LL0¼ 1 þ uz;z
kr¼ll0¼ 1 þ eAtt
ð11Þ As the volume is supposed to remain constant, the initial and ﬁnal radial positions of each component can be related by the following expression:
If a0is the lay angle of this component in the initial state, one has:
since after deformation the pitch length, P, determined by P = P0kz, the corresponding lay angle a in the
de-formed state is given by tan a¼tan a0
Let us consider a structure having the initial length L0, and bounded by planes perpendicular to the
struc-ture axis. The initial length of a component of lay angle a0is
l0¼ L0=cos a0 ð15Þ
the axial length in the deformed state being kzL0, the corresponding component length in the deformed state is
l¼ ðkzL0Þ= cos a ð16Þ
using Eqs. (13)–(16), the component extension ratio kr can be expressed as follows:
k2r¼ kz cos a0 cos a 2 ¼ k2zcos 2a 0þ sin2a0 kz ð17Þ which yields eA tt from (11)2. 4.1.2. Rotation
When the structure undergoes a relative rotation, hz, between the two end sections of length L0, the axial
strain of the component due to this rotation is expressed by eR
ð18Þ where Dl is deﬁned by (see Fig. 7(b))
Dl¼ rhzsin a ð19Þ
substituting (12 ), (15 ) and (19) into expression (18), we obtain: eRtt ¼ r0ﬃﬃﬃﬃ
p hz;zsin a cos a0 ð20Þ
where hz,zis the twist angle per unit length deﬁned by
ð21Þ However, in general, for a given structure, its outer diameter, reo, is known, as well as the value of the lay angle
on the outer layer, aeo. Since for all the components the pitch length, P, is the same, the lay angle of an arbitrary
component with a radial position of ro, can be written as a function of the parameters of the outer layer:
tan ao ¼
tan aeo ð22Þ
using Eqs. (14) and (22), one obtains:
cos2a¼ r 2 eok 3 z r2 eok 3 zþ r2otan2aeo sin2a¼ r 2 0tan 2a eo r2 eok 3 zþ r2otan 2a eo 8 > > > < > > > : ð23Þ
While taking into account the expressions (11) and substituting relations (17) and (20) into Eq. (10), the total axial strain of the component is given by
ett ¼ eAtt þ e R tt ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ k2zcos2a oþ sin2ao kz s 1 2 4 3 5 þ ro ﬃﬃﬃﬃ kz p hz;zsin a cos ao ð24Þ
where sin a is given according to Eq. (23)2, which are functions of extension ratio, kz, and the outer layer
parameters associated to the initial geometry (reoand aeo). Otherwise, cos aoand sin aoare given by
substitut-ing kz= 1 into the relation (23). Therefore, for an arbitrary point at a radial position ro, the axial strain in the
local coordinate system, ett, is a function of two independent variables, kzand ro.
4.2. Stiﬀness matrix derivation
In this model the components are assumed to be purely tensile elements with a uniaxial behavior that can be represented by
rtt ¼ Eett ð25Þ
where t is the tangent to the component centerline (see Fig. 5). In order to obtain the stiﬀness matrix the stress
in the local coordinate system, rtt, is transformed to the global cylindrical coordinate system (r, h, z):
rzz ¼ rttcos2a
rzh¼ rttcos a sin a
ð26Þ therefore, the total axial force and torque are obtained by integration of the stresses on the cross-section area of the structure in the initial state:
Fz¼ PFg R2p 0 Rreo 0 rttcos 2a r odrodh Mz¼ PFg R2p 0 Rreo 0 rttcos a sin ar 2 odrodh ( ð27Þ
where rttis obtained from (24) and (25) and cos a and sin a from (23). The global packing factor (PFg) is
intro-duced to take into account the presence of the voids in the whole of the cross-sectional area of the structure. It can be expressed by PFg¼ NAc R2p 0 Rreo 0 rodrodh R2p 0 Rreo 0 cos aorodrodh " #, ðpr2 eoÞ ð28Þ
where N is the total number of components in the structure.
After integration of the relations (27) using the MapleTMsoftware, and rewriting the results in the matrix
kee¼ 2pEcr2eoPFgk 2:5 z ln 1 2þ tan 2 aeoþ k3z 2 þ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð1 þ tan2a eoÞðk3zþ tan 2a eoÞ q tan2aeoðkz 1Þ 2 6 6 4 ﬃﬃﬃﬃ kz p lnðk3zþ tan 2a eoÞ þ ln 12þk 3 z 2 þ k 1:5 z ﬃﬃﬃﬃkz p lnðk3zÞ tan2a eoðkz 1Þ 3 5 keh¼ 2pEcr3eoPFgk4:5z lnðk3 zþ tan 2a eoÞ þ k3z ðk3 zþ tan 2a eoÞ lnðk3 zÞ 1 tan3a eo 2 6 6 6 4 3 7 7 7 5 khe¼23pEcr3eoPFg 1 4kzð1 k 3 zÞ ln 1 2þ tan 2a eoþ k3z 2 þ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð1 þ tan2a eoÞðk3zþ tan 2a eoÞ q þ2 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃð1 þ tan2a eoÞðk 3 zþ tan 2a eoÞ q 1 2k 1:5 z ðtan 2 aeo k 3 zlnðk 3 zþ tan 2 aeoÞÞ 1 4kzð1 k 3 zÞ ln 1 2þ k3z 2 þ k 1:5 z þ 2k1:5z 1 2k 4:5 z lnðk 3 zÞ =½tan3a eoðkz 1Þ khh¼23pEcr4eoPFgk3z tan2a eo k6z k3zþ tan2a eo þ k3z 2k3zðlnðk3zþ tan2 aeoÞ lnðk3zÞÞ " # tan4a eo 8 > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > < > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > > : ð29Þ
the stiﬀness matrix is a function of only the extension ratio of the structure, kz, global packing factor, PFg, and
the outer layer geometrical parameters of the structure in the initial state (reoand aeo). Since the stiﬀness
ma-trix components depend on the strain, this model is essentially non-linear, but for the interval [1.001 1.04] of
extension ratio (practical strain range for aramid), kz, the results can be considered as constant. In the
follow-ing, the results for the same axial strain (kz= 1.01) are presented.
5. Models comparison
The previous models have been applied to a strand of a 205 ton aramid cable of known construction parameters (given by the cable supplier) shown in Table 1.
Available construction parameters for strand of 205 T aramid cable
Outer diameter 18.3 (mm)
Pitch length 275 (mm)
Components number 42
Component axial stiﬀness, kc a
346.1 kN a k
cobtained from experiments.
Necessary input data for all models Models Input data
Raoof and Hoppe Pitch length, number of layers, components number per layer, component radius, Young’s modulus of component Leech Pitch length, number of layers, component number per layer, components radius, component axial stiﬀness, kc, PF
for each layer
Table 2 shows the input data necessary for all models.
Comparing Tables 1 and 2 shows that input data are missing for all the models. A sensitivity analysis has been performed elsewhere by Ghoreishi (2005), and the results have shown that the overall behavior is not sensitive to these missing values for the practical structures of interest here (aeo615). Some illustrative parts
of this sensitivity analysis are reported hereafter.
As it has been previously mentioned, it is practically diﬃcult to represent the strand cross-section with a multilayered structure. Therefore, several multilayered discretizations can be a priori deﬁned. From the value of the strand radius and assembled yarn surface, it has been considered that the strand was made with four layers. The results obtained with the Leech’s model corresponding to three diﬀerent multilayered discretiza-tions are given in Table 3, with very small diﬀerences.
The inﬂuence of the packing factor has also been studied, since this parameter is not deﬁned at the local scale (i.e. in each layer) when the Leech’s model is used. A four layers discretization with respectively 1, 6, 14 and 21 assembled yarns in each layer, has been considered, with three diﬀerent values of the radius of the assembled yarn. For a given value of this radius, the packing factor of the layers 2–4 was constant and calibrated in order to obtain a cross-section radius consistent with the strand radius value. The results are listed in Table 4, where it can be checked that they are slightly sensitive to the packing factor values.
Therefore, for the present study, the values for the missing data were taken as follows: Number of layers is chosen to be 4.
Component numbers for each layer are 1, 6, 14 and 21 and the PF in each layer are 1, 0.75, 0.88 and 0.89 respectively.
On the other hand, Eq. (28) gives a global packing factor, PFg= 0.86. This value is in agreement with the
previous values used in the Leech’s model, which shows that both models have the same quantity of material in the cross-section of the structure.
Results obtained for Leech’s model for diﬀerent multilayer discretizations of the strand made of 42 assembled yarns distributed in four layers Multilayered discretization kee(10 3 kN) keh(kN m) khe(kN m) khh(N m 2 ) 1 + 6 + 14 + 21 14.1 13.3 13.0 21.7 1 + 7 + 14 + 20 14.1 13.1 12.8 21.4 3 + 8 + 13 + 18 14.1 13.0 12.7 21.5 Table 4
Results obtained for Leech’s model for diﬀerent values of Packing factor
Assembled yarn radius (mm) PF of layers 2–4 kee(103kN) keh(kN m) khe(kN m) khh(N m2)
1.31 0.866 14.1 13.3 13.0 21.7
1.35 0.921 14.1 12.9 12.7 21.1
1.38 0.958 14.1 12.9 12.7 21.0
Results obtained for diﬀerent models applied to the strand of 205 T aramid cable
Models kee(103kN) keh(kN m) khe(kN m) khh(N m2) kehkhekeh ð%Þ
Raoof Full slip 14.1 13.5 13.7 19.0 1.48
No-slip 14.7 7.72 9.27 105 20 Hoppe 14.1 – – – – Leech l= 0 14.1 13.3 13.0 21.7 2.26 l= 0.15 14.1 13.3 13.5 22.1 1.50 l= 0.3 14.2 13.4 13.9 22.9 3.73 Continuum model 14.1 13.2 13.1 16.5 0.76
Component radius: 1.31 mm which yields a value of 6.42 104N/mm2for Young’s modulus of component. Table 5 presents the results obtained for the diﬀerent models. Besides the calculated stiﬀness matrix
com-ponents, the percentage of asymmetry between coupling terms, kehand khe, is shown for each model. The
inﬂu-ence of friction is presented for the Raoof and Leech models. It should be noted that in synthetic ﬁber ropes, the friction coeﬃcient between the diﬀerent components is not a well known parameter. For the yarn on yarn, and the aramid material, friction coeﬃcient values are given between 0.11 and 0.24 (FRM, 2003). These values have been obtained from tests on the diﬀerent yarns.
It should be also mentioned that, in Raoof’s model, the packing factor in each layer is assumed to bep
metallic components), but here this value is modiﬁed by using the value corresponding to that chosen in the
FRM software, as well as the global packing factor for the continuum model. Indeed, the same structure is deﬁned for all the models (same material quantity in the structure).
The main conclusion from Table 5 is that all the models yield very similar results for the axial stiﬀness, kee.
The diﬀerence for the coupling terms is visible. Only the torsion term results, khh, are signiﬁcantly diﬀerent for
the diﬀerent models.
To show which model gives more reliable results (particularly for the torsion term, khh), it would be
nec-essary to be able to compare them to experimental results.
In Raoof’s model, the structure in the no-slip case is much stiﬀer than in full-slip, however the coupling terms are smaller in the no-slip case. On the other hand, except for the axial stiﬀness where the two limit case results are similar, the diﬀerences between the two cases are signiﬁcant, particularly for the torsion term. It is interesting to note that the orthotropic sheet theory presented for the multilayered metallic cables by Raoof, and based on the contact theory between the metallic components with circular cross-section, yields results completely comparable with those obtained from other speciﬁc models for synthetic cables.
The model of Hoppe provides a similar value for the axial stiﬀness but does not allow the other stiﬀness terms to be obtained.
The results from Leech’s model show that the friction eﬀect can be neglected for axial loading. However, it should be mentioned that while the friction eﬀect plays a small role in global stiﬀness behavior of such struc-tures, the eﬀect of friction on the long-term performance and durability of a structure under cyclic loading can be signiﬁcant.
Then, the theoretical predictions will be compared to experimental results which are obtained from traction test on two diﬀerent structures.
6. Experimental results
Experimental studies have been performed at two scale levels, ﬁrst on yarns to determine the base compo-nent properties and then on two diﬀerent assembled yarns which represent the multilayer structure.
Tensile tests at the yarn level give an indication of the material behavior without the eﬀects of twist and construction. They were performed on a 10 kN test machine at an applied crosshead displacement rate of 50 mm/min. Elongation was measured using two digital cameras, which record the movements of marks on the yarns, as shown in Fig. 8. The test procedure for these and all subsequent tests was to apply ﬁve bed-ding-in load–unload cycles up to 50% of the nominal break load, before the load cycle which was used for the modeling. This is standard practice in rope testing and stabilizes the material and construction.
An example of the yarn test results including the ﬁve bedding-in cycles and the test to failure is shown in Fig. 9. 0 100 200 300 400 500 600 0 0.5 1 1.5 2 2.5 3
Chailleux and Davies (2003) have also used yarn tests to identify the intrinsic viscoelastic and viscoplastic behaviour of the aramid ﬁbers used in the present study (Twaron 1000).
In order to provide data for correlation with the models, tests were then performed on two diﬀerent assem-bled yarns taken from a 25 ton break load rope, Fig. 10 (at least ﬁve specimens were characterized for each), for which the construction parameters are given in Table 6. All the samples were made with the same aramid ﬁber grade. The load was introduced through cone and spike end connections. Tests involved applying ﬁve initial bedding-in cycles, as for the yarn tests, by loading the samples to 50% of their nominal break load at a loading and rate of 50 mm/min then unloading at the same rate. The same image analysis system was used, measuring the displacements of two marks bonded to the assembled yarn (Fig. 10). From the tests
on the component (yarn) and the structures (assembled yarns 1 and 2) the axial stiﬀness values were measured as shown in Table 7. The stiﬀness values presented are those from the 6th loading.
7. Comparison between prediction and tests
In this section the previous experimental results will be compared to models predictions. For modeling the assembled yarn 1, the number of layers is assumed to be 2, for which the component numbers for each layer are 3 and 9. The PF’s for each layer are both 0.95, and the corresponding global packing factor, from Eq. (28), is also 0.95. In the assembled yarn 2, the number of layers is assumed to be 3 in which the component numbers for each layer are 1, 5 and 10. The PF’s in each layer are 1, 0.96 and 0.96 respectively and the corresponding global packing factor, from Eq. (28), is 0.96.
The yarn axial stiﬀness and the geometrical parameters then enable a prediction to be made of the stiﬀness
coeﬃcients of the structures using the continuum model (Eq. (29)1), and this gives axial stiﬀness values of
252.7 kN and 336.7 kN for assembled yarns 1 and 2 respectively. The structures were also modeled with the FRM software, and this gives results very close to those of the continuum model (252.6 kN and 336.9 kN respectively). Raoof’s model was not applied to these structures because there are not a large number of wires in each of the layers here.
The comparison is shown graphically in Fig. 11.
Construction parameters for diﬀerent structures
Structure Construction parameters Structure Construction parameters
Assembled yarn 1 Outer diameter 2.03 (mm) Assembled yarn 2 Outer diameter 2.33 (mm) Component diameter 0.572 (mm) Component diameter 0.572 (mm) Pitch length 52.6 (mm) Pitch length 58.8 (mm)
Component number 12 Component number 16
Component axial stiﬀness, kc 21.4 kN component axial stiﬀness, kc 21.4 kN
Test results on the yarns and assembled yarns after ﬁve bedding-in cycles
Samples Test number Sample length (mm) Average axial stiﬀness (kN) Average rupture force (kN) Yarn (Twaron 1000) 5 349–355 21.4 ± 1% 0.550 ± 2% Assembled yarn 1 6 344–352 228.2 ± 3.6% 5.12 ± 8% Assembled yarn 2 5 343–354 298.5 ± 0.8% 6.88 ± 14% 0 500 1000 1500 2000 2500 0 0.3 0.6 0.9 Axial strain (%) Axial force (N) Experiment Leech's model Continuum model 0 500 1000 1500 2000 2500 3000 0 0.3 0.6 0.9 Axial strain (%) Axial force (N) Experiment Leech's model Continuum model
Fig. 11. Comparison between present model predictions, FRM software results and corresponding experimental measurements for force– strain curve of (a) assembled yarn 1 and (b) assembled yarn 2.
So far all the tests performed have concentrated on the axial stiﬀness keeby testing structures with ﬁxed end
loading conditions. However, a small number of tests have shown that there is not measurable tension–torsion coupling terms and torsion stiﬀness for the small diameter assembled yarns at this level. In order to determine the other coeﬃcients (coupling terms and torsion term) and to compare them with predicted values test results for the higher level such as strands of 205 T ﬁber rope would be necessary.
A non-linear elastic continuum model has been developed for the analysis of the overall axial stiﬀness of ﬁbrous structures with a large number of twisted components. By contrast with multilayered approaches, the structure under consideration is herein depicted as a set of coaxial helixes only characterized by their exter-nal lay angle and corresponding radius. The constitutive material is assumed to be linear. Static monotonic axial loads are considered, the inter-ﬁber friction eﬀects are not taken into account. Moreover, the studied structures exhibiting small lay angles, the overall diametral contractions are neglected, which may contribute to the overestimation of stiﬀness. The analytical model developed leads to useful closed-form expressions thus allowing rope constructions to be optimized.
Due to lack of published experimental data, the model has ﬁrst been compared with models of the litera-ture. The results obtained, have shown that all the models give results that agree reasonably well with each other, except with respect to the torsion stiﬀness, for which there is a signiﬁcant diﬀerence. In addition, stiﬀ-ness matrices of all the models deviate slightly from symmetry and this lack of symmetry is due to a certain lack of consistency in the various simplifying hypotheses.
Tensile tests have then been performed on aramid ﬁber assemblies with two structures, to obtain the axial stiﬀness. The preliminary test results indicate a good correlation with the model. Additional test data, espe-cially to examine tension–torsion and pure torsion loading, are needed to gauge performance of the models. The integration of these results in a model for a large aramid wire rope and comparison with tension and ten-sion–torsion coupling test results will be described in Part II (Ghoreishi et al., in press) of this paper.
Beltran, J.F., Rungamornrat, J., Williamson, E.B., 2003. Computational model for the analysis of damage ropes. In: Proceedings of The thirteenth International Oﬀshore and Polar Engineering Conference, Honolulu, Hawai, USA.
Beltran, J.F., Williamson, E.B., 2004. Investigation of the damage-dependent response of mooring ropes. In: Proceedings of The Fourteenth International Oﬀshore and Polar Engineering Conference Toulon, France.
Blouin, F., Cardou, A., 1989. A study of helically reinforced cylinders under axially symmetric loads mathematical modelling. International Journal of Solids and Structures. 25 (2), 189–200.
Chailleux, E., Davies, P., 2003. Modelling the non-linear viscoelastic and viscoplastic behaviour of aramid ﬁber yarns. Mechanics of Time Dependent Materials Journal 7 (3–4), 291–303.
Crossley, J.A., Spencer, A.J.M., England, A.H., 2003a. Analytical solutions for bending and ﬂexure of helically reinforced cylinders. International Journal of Solids and Structures 40 (4), 777–806.
Crossley, J.A., England, A.H., Spencer, A.J.M., 2003b. Bending and ﬂexure of cylindrically monoclinic elastic cylinders. International Journal of Solids and Structures 40 (25), 6999–7013.
Foster, G.P., 2002. Advantages of ﬁber rope over wire rope. Journal of Industrial Textiles 32 (1), 67–75.
FRM, Fibre Rope Modeller, version 1.1.5, 2003. Software development for Tension Technology International Ltd. (TTI).
Ghoreishi, S.R., 2005. Mode´lisation analytique et caracte´risation expe´rimentale du comportement de caˆbles synthe´tiques. Ph.D. Thesis, Ecole Centrale de Nantes, France.
Ghoreishi, S.R., Davies, P., Cartraud, P., Messager, T., in press. Analytical modeling of synthetic ﬁber ropes, part II: A linear elastic model for 1 + 6 ﬁbrous structures. International Journal of Solids and Structures, doi:10.1016/j.ijsolstr.2006.08.032.
Hobbs, R.E., Raoof, M., 1982. Interwire slippage and fatigue prediction in stranded cables for TLP tethersBehaviour of Oﬀshore Structures, 2. Hemisphere publishing/McGraw-Hill, New York, pp. 77–99.
Hoppe, L.F.E., 1991. Modeling the Static Behavior of Dyneema in Wire-rope Construction. MTS RTM.
Jolicoeur, C., Cardou, A., 1994. An analytical solution for bending of coaxial orthotropic cylinders. Journal of Engineering Mechanics 120 (12), 2556–2574.
Jolicoeur, C., Cardou, A., 1996. Semicontinuous mathematical model for bending of multilayered wire strands. Journal of engineering Mechanics 122 (7), 643–650.
Leech, C.M., Hearle, J.W.S., Overington, M.S., Banﬁeld, S.J., 1993. Modelling tension and torque properties of ﬁbre ropes and splices. In: Proceeding of the Third International Oﬀshore and Polar Engineering Conference Singapore.
Mindlin, R.D., 1949. Compliance of elastic bodies in contact. Journal of Applied Mechanics 16, 259–268.
Raoof, M., 1983. Interwire contact forces and the static, hysteretic and fatigue properties of multi-layer structural strands. Ph.D. Thesis, Imperial College of Science and Technology, London, UK.
Raoof, M., 1991. Method for analysing large spiral strands. Journal of Strain Analysis 26 (3), 165–174.
Raoof, M., Hobbs, R.E., 1988. Analysis of multilayered structural strands. Journal of engineering Mechanics 114 (7), 1166–1182. Raoof, M., Kraincanic, I., 1995a. Simple derivation of the stiﬀness matrix for axial/torsional coupling of spiral strands. Computers and
Structures 55 (4), 589–600.
Raoof, M., Kraincanic, I., 1995b. Analysis of large diameter steel ropes. Journal of Engineering Mechanics 121 (6), 667–675.
Rungamornrat, J., Beltran, J.F., Williamson, E.B., 2002. Computational model for synthetic-ﬁber rope response. In: Proceeding of Fifteenth Engineering Mechanics Conference. ASCE, New York.